3 Sample selection The nine natural volcanic glasses used were fresh, unweathered, unaltered, and nonhydrated obsidians free of cracks with low crystal (< 1%) and bubble content (< 1%). Chemical composition of the matrix glass was quantified by electron microanalysis (SEM-EDX, DSM 940 CARL ZEISS, eXL 10 Spektrometer, Oxford Instruments). Volatile- species and thus water content are determined in high-vacuum degassing experiments (controlled heating rate 10K/min from RT-1500C) coupled with a quadropole mass spectrometer (QMA 125 Balzers, Schmidt and Heide (2000), Leschik et al. (2003), Heide and Schmidt (2003)). Y EL is a grey crystal-poor obsidian from Yellowstone (USA). V UL from Vulcano, LIP from Lipari (Italy) and JAL from Jalisco (Mexico) are grey crystalfree glasses. The sample MIL from Milos (Greek) is grey-black crystal- poor. RAB from Hrafntinnuhryggur (Island) and DY R from Artenis (Armenia) are black crystal-poor glasses. The obsidian ATS from Artis (Armenia) is grey crystal- poor with crystal bands. QUI from Quironcolo (Argentinia) and IKI from Ikizidre (Turkey) are transparent homogeneous obsidians with very few large crystals. 4 Experiments ~1m furance tensile unloading system thin tantal layer d=0.03mm free flexure mode oscillations fixed free pendulums rod NCT3-steel pendulum‘s weight displacement sensor system glass sample Fig. 4. Flexure Pendulum Equipment. The flexure pendulum is shown in Fig. 4. It operates in air at a frequency of about 0.63Hz (small deformations ≈ 10 −5 ...10 −3 ) and temperatures up to T ≈ 1000 ◦ C (cf. Bark-Zollmann (1994), Bark-Zollmann et al. (1997a), Bark-Zollmann et al. (1997b), Bark-Zollmann et al. (1998a), 14 20mm 40mm
Table 3 Chemical composition and water-content (wt.%) of the volcanic glasses.